Crystal chemistry of the M2+[(UO2)(T6+O4)2(H2O)](H2O)4 (M2+ = Mg, Mn, Fe, Co, Ni and Zn; T6+ = S, Se) compounds: the interplay between chemical composition, pH and structural architecture
Kornyakov, Ilya V.; Tyumentseva, Olga S.; Krivovichev, Sergey V.; Tananaev, Ivan G.; Gurzhiy, Vladislav V.; CrystEngComm 23 (2021) 1140–1148; doi:10.1039/D0CE01587C

data_7241874
_publ_section_title
;
 Crystal chemistry of the M2+[(UO2)(T6+O4)2(H2O)](H2O)4 (M2+ = Mg, Mn, Fe,
 Co, Ni and Zn; T6+ = S, Se) compounds: the interplay between chemical
 composition, pH and structural architecture
;
_journal_issue                   5
_journal_name_full               CrystEngComm
_journal_page_first              1140
_journal_page_last               1148
_journal_paper_doi               10.1039/D0CE01587C
_journal_volume                  23
_journal_year                    2021
_chemical_formula_moiety         'H10 Ni O15 S2 U'
_chemical_formula_sum            'H10 Ni O15 S2 U'
_chemical_formula_weight         610.94
_space_group_crystal_system      orthorhombic
_space_group_IT_number           31
_space_group_name_Hall           'P 2ac -2'
_space_group_name_H-M_alt        'P m n 21'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     dual
_audit_creation_date             2020-10-18
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_audit_update_record
;
2020-10-18 deposited with the CCDC.	2020-12-08 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.75060(10)
_cell_length_b                   8.30950(10)
_cell_length_c                   11.29290(10)
_cell_measurement_reflns_used    34708
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      44.7710
_cell_measurement_theta_min      2.3930
_cell_volume                     1196.50(2)
_computing_cell_refinement       'CrysAlisPro 1.171.40.53 (Rigaku OD, 2019)'
_computing_data_collection       'CrysAlisPro 1.171.40.53 (Rigaku OD, 2019)'
_computing_data_reduction        'CrysAlisPro 1.171.40.53 (Rigaku OD, 2019)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      296(2)
_diffrn_detector                 'CCD plate'
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  t~exp~   \w     \q     \k     \f   Frames
  1  \w   -114.71 -28.21   0.50   10.00    --  -52.00 166.02 179.99  173
  2  \f      5.23 264.73   0.50   10.00 -39.40 -52.00 102.00    --   519
  3  \f   -295.60 -31.10   0.50   10.00 -34.45 -38.00 161.98    --   529
  4  \f   -200.27   6.73   0.50   10.00 -74.17 -44.00-156.00    --   414
  5  \w    -82.44  -8.44   0.50   10.00    --  -48.00 117.99 132.01  148
  6  \f     16.09 272.09   0.50   10.00 -42.45 -36.00 167.96    --   512
  7  \w    -78.16 -24.16   0.50   10.00    --  -44.00  99.99 -30.00  108
  8  \f    153.84 293.34   0.50   10.00-131.49 -54.00 -93.99    --   279
  9  \w    229.47 302.47   0.50   10.00    --  -46.00 -60.00  70.00  146
 10  \f   -359.99   9.51   0.50   10.00 -63.55 -36.00 137.99    --   739
 11  \w    238.20 278.70   0.50   10.00    --  -44.00 -92.00  46.00   81
 12  \w    -68.48  -6.98   0.50   10.00    --  -52.00 106.00  36.00  123
 13  \f    156.99 260.49   0.50   10.00 -92.21 -44.00-109.99    --   207
;
_diffrn_measurement_device       'abstract diffractometer'
_diffrn_measurement_device_type
'Saxi-CrysAlisPro-abstract goniometer imported SAXI images'
_diffrn_measurement_method       '\w and \f scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0051957000
_diffrn_orient_matrix_UB_12      0.0849933000
_diffrn_orient_matrix_UB_13      -0.0013552000
_diffrn_orient_matrix_UB_21      -0.0546274000
_diffrn_orient_matrix_UB_22      -0.0081358000
_diffrn_orient_matrix_UB_23      -0.0103285000
_diffrn_orient_matrix_UB_31      -0.0092751000
_diffrn_orient_matrix_UB_32      0.0004482000
_diffrn_orient_matrix_UB_33      0.0618945000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0504
_diffrn_reflns_av_unetI/netI     0.0140
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            28646
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.490
_diffrn_reflns_theta_min         2.409
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    15.521
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.14111
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.40.53 (Rigaku Oxford Diffraction, 2019)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'clear yellowish green'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   yellowish
_exptl_crystal_colour_primary    green
_exptl_crystal_density_diffrn    3.392
_exptl_crystal_description       plate
_exptl_crystal_F_000             1128
_exptl_crystal_size_max          0.37
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.1
_refine_diff_density_max         1.732
_refine_diff_density_min         -1.337
_refine_diff_density_rms         0.260
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.965(13)
_refine_ls_extinction_coef       0.0013(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.128
_refine_ls_hydrogen_treatment    refxyz
_refine_ls_matrix_type           full
_refine_ls_number_parameters     219
_refine_ls_number_reflns         2150
_refine_ls_number_restraints     31
_refine_ls_restrained_S_all      1.165
_refine_ls_R_factor_all          0.0282
_refine_ls_R_factor_gt           0.0277
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0592P)^2^+0.3756P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0752
_refine_ls_wR_factor_ref         0.0758
_reflns_Friedel_coverage         0.905
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     1.000
_reflns_number_gt                2092
_reflns_number_total             2150
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d0ce01587c1.cif
_cod_data_source_block           Compound_1
_cod_depositor_comments
'Adding full bibliography for 7241870--7241883.cif.'
_cod_database_code               7241874
_shelxl_version_number           2014/6
_chemical_oxdiff_formula         'Ni4  O60  S8  U4  '
_shelx_estimated_absorpt_t_max   0.306
_shelx_estimated_absorpt_t_min   0.069
_reflns_odcompleteness_completeness 94.28
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     44.68
_olex2_refinement_description
;
1. Twinned data refinement
 Scales: 0.035(13)
 0.965(13)
2. Fixed Uiso
 At 1.5 times of:
  All O(H) groups, All O(H,H) groups, All O(H,H,H) groups
3. Restrained distances
 O12-H12_$1
 0.98 with sigma of 0.02
 H12-H12_$1
 1.54 with sigma of 0.02
 H12_$1-O4_$6
 2 with sigma of 0.02
 O10_$1-H14_$6
 2.1 with sigma of 0.02
 O14-H14_$1
 0.98 with sigma of 0.02
 H14-H14_$1
 1.54 with sigma of 0.02
 H14_$7-O10_$6
 1.9 with sigma of 0.02
 O10_$6-H10B_$6
 0.98 with sigma of 0.02
 H10B_$6-O7_$8
 1.8 with sigma of 0.02
 O10_$6-H10A_$6
 0.98 with sigma of 0.02
 H10B_$6-H10A_$6
 1.54 with sigma of 0.02
 H10A_$6-O4_$9
 1.8 with sigma of 0.02
 O16_$7-H16_$10
 0.98 with sigma of 0.02
 H16_$7-H16_$10
 1.54 with sigma of 0.02
 H16_$7-O3_$9
 1.9 with sigma of 0.02
 O15_$8-H15_$11
 0.98 with sigma of 0.02
 H15_$8-H15_$11
 1.54 with sigma of 0.02
 H15_$11-O5_$2
 1.9 with sigma of 0.02
 H12_$8-O4_$9
 1.8 with sigma of 0.02
 O13-H13_$1
 0.98 with sigma of 0.02
 O19-H19
 0.98 with sigma of 0.02
 H19_$5-H19
 1.54 with sigma of 0.02
 H19-O5_$4
 1.75 with sigma of 0.02
 O17-H17
 0.98 with sigma of 0.02
 H17-H17_$5
 1.54 with sigma of 0.02
 H17-O11_$3
 2.3 with sigma of 0.02
 H13-H13_$1
 1.54 with sigma of 0.02
 O18-H18
 0.98 with sigma of 0.02
 H18-H18_$5
 1.54 with sigma of 0.02
 O3_$5-H18_$5
 2.4 with sigma of 0.02
;
_shelx_res_checksum              25834
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
- Detector area scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 3.280
_oxdiff_exptl_absorpt_empirical_full_min 0.521